Abstract
Bulk laser damage variability in deuterated potassium dihydrogen phosphate (DKDP) crystals is well known and makes online conditioning of multiplebeam laser systems difficult to optimize. By using an empirical model, called Absorption Distribution Model (ADM), we were able to map the damage variability of the crystals (boule to boule as well as within same boule) in terms of defect population variations. The defect population variation was found to coalesce into two distinct groupings that can be identified by the defect population in the late growth region of the boule. This result allows us to optimize the conditioning protocol for an arbitrary number of beams with crystals of differing damage quality.
© 2012 OSA
Full Article  PDF ArticleOSA Recommended Articles
Zhi M. Liao, M. L. Spaeth, K. Manes, J. J. Adams, and C. W. Carr
Opt. Lett. 35(15) 25382540 (2010)
Paul DeMange, Raluca A. Negres, Christopher W. Carr, Harry B. Radousky, and Stavros G. Demos
Opt. Express 14(12) 53135328 (2006)
Zhi M. Liao, B. Raymond, J. Gaylord, R. Fallejo, J. Bude, and P. Wegner
Opt. Express 22(23) 2884528856 (2014)
References
 View by:
 Article Order
 
 Year
 
 Author
 
 Publication
 P. Wegner, J. Auerbach, T. Biesiada, S. Dixit, J. Lawson, J. Menapace, T. Parham, D. Swift, P. Whitman, and W. Williams, “NIF final optics systems: frequency conversion and beam conditioning,” Proc. SPIE 5341, 180–189 (2004).
[Crossref]  J. Swain, S. Stokowski, D. Milam, and F. Rainer, “Improving the bulk laser damage resistance of potassium dihydrogen phosphate crystals by pulsed laser irradiation,” Appl. Phys. Lett. 40(4), 350–352 (1982).
[Crossref]  J. J. Adams, C. W. Carr, M. D. Feit, A. M. Rubenchik, M. L. Spaeth, and R. P. Hackel, “Pulse length dependence of laser conditioning and bulk damage in KD2PO4,” Proc. SPIE 5647, 265 (2004).
 M. Runkel, K. Neeb, M. Staggs, J. Auerbach, and A. Burnham, “Results of raster scan laser conditioning studies on DKDP triplers using Nd:YAG and excimer lasers,” Proc. SPIE 4679, 348 (2001).
 M. Runkel and A. K. Burnham, “Difference in bulk damage probability distributions between tripler and zcuts of KDP and DKDP at 355nm,” Proc. SPIE 4347, 408 (2000).
 A. K. Burnham, M. Runkel, R. A. HawleyFedder, M. L. Carman, R. A. Torres, and P. K. Whitman, “Lowtemperature growth of DKDP for improving laserinduced damage resistance at 350nm,” Proc. SPIE 4347, 373 (2000).
 S. G. Demos, M. Staggs, M. Yan, H. B. Radousky, and J. J. De Yoreo, “Investigation of optically active defect clusters in KH2PO4 under laser photoexcitation,” J. Appl. Phys. 85(8), 3988–3992 (1999).
[Crossref]  M. Yan, R. Torres, M. Runkel, B. Woods, I. Hutcheon, N. Zaitseva, and J. DeYoreo, “Investigation of impurity and laserinduced damage in the growth sectors of rapidly grown KDP crystals,” Proc. SPIE 2966, 11–16 (1997).
[Crossref]  M. Pommiès, D. Damiani, B. Bertussi, J. Capoulade, H. Piombini, J. Y. Natoli, and H. Mathis, “Detection and characterization of absorption heterogeneities in KH2PO4 crystals,” Opt. Commun. 267(1), 154–161 (2006).
[Crossref]  R. A. Negres, N. P. Zaitseva, P. DeMange, and S. G. Demos, “An expedited approach to evaluate the importance of different crystal growth parameters on laser damage performance in KDP and DKDP,” Proc. SPIE 6403, 64031S (2007).
 M. Runkel, M. Yan, J. De Yoreo, and N. Zaitseva, “The effect of impurities and stress on the damage distributions of rapidly grown KDP crystals,” Proc. SPIE 3244, 211 (1997).
 C. W. Carr, M. D. Feit, M. C. Nostrand, and J. J. Adams, “Techniques for qualitative and quantitative measurement of aspects of laserinduced damage important for laser beam propagation,” Meas. Sci. Technol. 17(7), 1958–1962 (2006).
[Crossref]  J. Adams, J. A. Jarboe, M. Feit, and R. P. Hackel, “Comparison between S/1 and R/1 tests and damage density vs. fluence (rho(phi)) results for unconditioned and subnanosecond laserconditioned KD2PO4 crystals,” Proc. SPIE 6720, 672014 (2008).

Z. M. Liao, M. L. Spaeth, K. Manes, J. J. Adams, and C. W. Carr, “Predicting laserinduced bulk damage and conditioning for deuterated potassium dihydrogen phosphate crystals using an absorption distribution model,” Opt. Lett. 35(15), 2538–2540 (2010).
[Crossref] [PubMed]  M. Spaeth, “Absorption distribution model,” LLNL Internal Presentation (2007).
 C. W. Carr, J. D. Bude, and P. DeMange, “Lasersupported solidstate absorption fronts in silica,” Phys. Rev. B 82(18), 184304 (2010).
[Crossref]  M. D. Feit and A. M. Rubenchik, “Implications of nanoabsorber initiators for damage probability curves, pulselength scaling and laser conditioning,” Proc. SPIE 5273, 74–82 (2003).
 J. B. Trenholme, M. D. Feit, and A. M. Rubenchik, “Sizeselection initiation model extended to include shape and random factors,” Proc. SPIE 5991, 59910X (2005).
[Crossref]  M. Runkel, M. Yan, J. De Yoreo, and N. Zaitseva, “The effect of impurities and stress on the damage distributions of rapidly grown KDP crystals,” Proc. SPIE 3244, 211 (1997).
 M. Runkel, J. Bruere, W. Sell, T. Weiland, D. Milam, D. Hahn, and M. Nostrand, “Effects of pulse duration of bulk laser damage in 350nm rasterscanned DKDP,” Proc. SPIE 4392, 405 (2002).
 C. W. Carr, J. B. Trenholme, and M. L. Spaeth, “Effect of temporal pulse shape on optical damage,” Appl. Phys. Lett. 90(4), 041110 (2007).
[Crossref] 
Z. M. Liao, J. Huebel, J. Trenholme, K. Manes, and C. W. Carr, “Modeling maxofN fluence distribution using measured shottoshot beam contrast,” Appl. Opt. 50(20), 3547–3552 (2011).
[Crossref] [PubMed]
2011 (1)
Z. M. Liao, J. Huebel, J. Trenholme, K. Manes, and C. W. Carr, “Modeling maxofN fluence distribution using measured shottoshot beam contrast,” Appl. Opt. 50(20), 3547–3552 (2011).
[Crossref]
[PubMed]
2010 (2)
Z. M. Liao, M. L. Spaeth, K. Manes, J. J. Adams, and C. W. Carr, “Predicting laserinduced bulk damage and conditioning for deuterated potassium dihydrogen phosphate crystals using an absorption distribution model,” Opt. Lett. 35(15), 2538–2540 (2010).
[Crossref]
[PubMed]
C. W. Carr, J. D. Bude, and P. DeMange, “Lasersupported solidstate absorption fronts in silica,” Phys. Rev. B 82(18), 184304 (2010).
[Crossref]
2008 (1)
J. Adams, J. A. Jarboe, M. Feit, and R. P. Hackel, “Comparison between S/1 and R/1 tests and damage density vs. fluence (rho(phi)) results for unconditioned and subnanosecond laserconditioned KD2PO4 crystals,” Proc. SPIE 6720, 672014 (2008).
2007 (2)
R. A. Negres, N. P. Zaitseva, P. DeMange, and S. G. Demos, “An expedited approach to evaluate the importance of different crystal growth parameters on laser damage performance in KDP and DKDP,” Proc. SPIE 6403, 64031S (2007).
C. W. Carr, J. B. Trenholme, and M. L. Spaeth, “Effect of temporal pulse shape on optical damage,” Appl. Phys. Lett. 90(4), 041110 (2007).
[Crossref]
2006 (2)
M. Pommiès, D. Damiani, B. Bertussi, J. Capoulade, H. Piombini, J. Y. Natoli, and H. Mathis, “Detection and characterization of absorption heterogeneities in KH2PO4 crystals,” Opt. Commun. 267(1), 154–161 (2006).
[Crossref]
C. W. Carr, M. D. Feit, M. C. Nostrand, and J. J. Adams, “Techniques for qualitative and quantitative measurement of aspects of laserinduced damage important for laser beam propagation,” Meas. Sci. Technol. 17(7), 1958–1962 (2006).
[Crossref]
2005 (1)
J. B. Trenholme, M. D. Feit, and A. M. Rubenchik, “Sizeselection initiation model extended to include shape and random factors,” Proc. SPIE 5991, 59910X (2005).
[Crossref]
2004 (2)
P. Wegner, J. Auerbach, T. Biesiada, S. Dixit, J. Lawson, J. Menapace, T. Parham, D. Swift, P. Whitman, and W. Williams, “NIF final optics systems: frequency conversion and beam conditioning,” Proc. SPIE 5341, 180–189 (2004).
[Crossref]
J. J. Adams, C. W. Carr, M. D. Feit, A. M. Rubenchik, M. L. Spaeth, and R. P. Hackel, “Pulse length dependence of laser conditioning and bulk damage in KD2PO4,” Proc. SPIE 5647, 265 (2004).
2003 (1)
M. D. Feit and A. M. Rubenchik, “Implications of nanoabsorber initiators for damage probability curves, pulselength scaling and laser conditioning,” Proc. SPIE 5273, 74–82 (2003).
2002 (1)
M. Runkel, J. Bruere, W. Sell, T. Weiland, D. Milam, D. Hahn, and M. Nostrand, “Effects of pulse duration of bulk laser damage in 350nm rasterscanned DKDP,” Proc. SPIE 4392, 405 (2002).
2001 (1)
M. Runkel, K. Neeb, M. Staggs, J. Auerbach, and A. Burnham, “Results of raster scan laser conditioning studies on DKDP triplers using Nd:YAG and excimer lasers,” Proc. SPIE 4679, 348 (2001).
2000 (2)
M. Runkel and A. K. Burnham, “Difference in bulk damage probability distributions between tripler and zcuts of KDP and DKDP at 355nm,” Proc. SPIE 4347, 408 (2000).
A. K. Burnham, M. Runkel, R. A. HawleyFedder, M. L. Carman, R. A. Torres, and P. K. Whitman, “Lowtemperature growth of DKDP for improving laserinduced damage resistance at 350nm,” Proc. SPIE 4347, 373 (2000).
1999 (1)
S. G. Demos, M. Staggs, M. Yan, H. B. Radousky, and J. J. De Yoreo, “Investigation of optically active defect clusters in KH2PO4 under laser photoexcitation,” J. Appl. Phys. 85(8), 3988–3992 (1999).
[Crossref]
1997 (3)
M. Yan, R. Torres, M. Runkel, B. Woods, I. Hutcheon, N. Zaitseva, and J. DeYoreo, “Investigation of impurity and laserinduced damage in the growth sectors of rapidly grown KDP crystals,” Proc. SPIE 2966, 11–16 (1997).
[Crossref]
M. Runkel, M. Yan, J. De Yoreo, and N. Zaitseva, “The effect of impurities and stress on the damage distributions of rapidly grown KDP crystals,” Proc. SPIE 3244, 211 (1997).
M. Runkel, M. Yan, J. De Yoreo, and N. Zaitseva, “The effect of impurities and stress on the damage distributions of rapidly grown KDP crystals,” Proc. SPIE 3244, 211 (1997).
1982 (1)
J. Swain, S. Stokowski, D. Milam, and F. Rainer, “Improving the bulk laser damage resistance of potassium dihydrogen phosphate crystals by pulsed laser irradiation,” Appl. Phys. Lett. 40(4), 350–352 (1982).
[Crossref]
Adams, J.
J. Adams, J. A. Jarboe, M. Feit, and R. P. Hackel, “Comparison between S/1 and R/1 tests and damage density vs. fluence (rho(phi)) results for unconditioned and subnanosecond laserconditioned KD2PO4 crystals,” Proc. SPIE 6720, 672014 (2008).
Adams, J. J.
Z. M. Liao, M. L. Spaeth, K. Manes, J. J. Adams, and C. W. Carr, “Predicting laserinduced bulk damage and conditioning for deuterated potassium dihydrogen phosphate crystals using an absorption distribution model,” Opt. Lett. 35(15), 2538–2540 (2010).
[Crossref]
[PubMed]
C. W. Carr, M. D. Feit, M. C. Nostrand, and J. J. Adams, “Techniques for qualitative and quantitative measurement of aspects of laserinduced damage important for laser beam propagation,” Meas. Sci. Technol. 17(7), 1958–1962 (2006).
[Crossref]
J. J. Adams, C. W. Carr, M. D. Feit, A. M. Rubenchik, M. L. Spaeth, and R. P. Hackel, “Pulse length dependence of laser conditioning and bulk damage in KD2PO4,” Proc. SPIE 5647, 265 (2004).
Auerbach, J.
P. Wegner, J. Auerbach, T. Biesiada, S. Dixit, J. Lawson, J. Menapace, T. Parham, D. Swift, P. Whitman, and W. Williams, “NIF final optics systems: frequency conversion and beam conditioning,” Proc. SPIE 5341, 180–189 (2004).
[Crossref]
M. Runkel, K. Neeb, M. Staggs, J. Auerbach, and A. Burnham, “Results of raster scan laser conditioning studies on DKDP triplers using Nd:YAG and excimer lasers,” Proc. SPIE 4679, 348 (2001).
Bertussi, B.
M. Pommiès, D. Damiani, B. Bertussi, J. Capoulade, H. Piombini, J. Y. Natoli, and H. Mathis, “Detection and characterization of absorption heterogeneities in KH2PO4 crystals,” Opt. Commun. 267(1), 154–161 (2006).
[Crossref]
Biesiada, T.
P. Wegner, J. Auerbach, T. Biesiada, S. Dixit, J. Lawson, J. Menapace, T. Parham, D. Swift, P. Whitman, and W. Williams, “NIF final optics systems: frequency conversion and beam conditioning,” Proc. SPIE 5341, 180–189 (2004).
[Crossref]
Bruere, J.
M. Runkel, J. Bruere, W. Sell, T. Weiland, D. Milam, D. Hahn, and M. Nostrand, “Effects of pulse duration of bulk laser damage in 350nm rasterscanned DKDP,” Proc. SPIE 4392, 405 (2002).
Bude, J. D.
C. W. Carr, J. D. Bude, and P. DeMange, “Lasersupported solidstate absorption fronts in silica,” Phys. Rev. B 82(18), 184304 (2010).
[Crossref]
Burnham, A.
M. Runkel, K. Neeb, M. Staggs, J. Auerbach, and A. Burnham, “Results of raster scan laser conditioning studies on DKDP triplers using Nd:YAG and excimer lasers,” Proc. SPIE 4679, 348 (2001).
Burnham, A. K.
M. Runkel and A. K. Burnham, “Difference in bulk damage probability distributions between tripler and zcuts of KDP and DKDP at 355nm,” Proc. SPIE 4347, 408 (2000).
A. K. Burnham, M. Runkel, R. A. HawleyFedder, M. L. Carman, R. A. Torres, and P. K. Whitman, “Lowtemperature growth of DKDP for improving laserinduced damage resistance at 350nm,” Proc. SPIE 4347, 373 (2000).
Capoulade, J.
M. Pommiès, D. Damiani, B. Bertussi, J. Capoulade, H. Piombini, J. Y. Natoli, and H. Mathis, “Detection and characterization of absorption heterogeneities in KH2PO4 crystals,” Opt. Commun. 267(1), 154–161 (2006).
[Crossref]
Carman, M. L.
A. K. Burnham, M. Runkel, R. A. HawleyFedder, M. L. Carman, R. A. Torres, and P. K. Whitman, “Lowtemperature growth of DKDP for improving laserinduced damage resistance at 350nm,” Proc. SPIE 4347, 373 (2000).
Carr, C. W.
Z. M. Liao, J. Huebel, J. Trenholme, K. Manes, and C. W. Carr, “Modeling maxofN fluence distribution using measured shottoshot beam contrast,” Appl. Opt. 50(20), 3547–3552 (2011).
[Crossref]
[PubMed]
Z. M. Liao, M. L. Spaeth, K. Manes, J. J. Adams, and C. W. Carr, “Predicting laserinduced bulk damage and conditioning for deuterated potassium dihydrogen phosphate crystals using an absorption distribution model,” Opt. Lett. 35(15), 2538–2540 (2010).
[Crossref]
[PubMed]
C. W. Carr, J. D. Bude, and P. DeMange, “Lasersupported solidstate absorption fronts in silica,” Phys. Rev. B 82(18), 184304 (2010).
[Crossref]
C. W. Carr, J. B. Trenholme, and M. L. Spaeth, “Effect of temporal pulse shape on optical damage,” Appl. Phys. Lett. 90(4), 041110 (2007).
[Crossref]
C. W. Carr, M. D. Feit, M. C. Nostrand, and J. J. Adams, “Techniques for qualitative and quantitative measurement of aspects of laserinduced damage important for laser beam propagation,” Meas. Sci. Technol. 17(7), 1958–1962 (2006).
[Crossref]
J. J. Adams, C. W. Carr, M. D. Feit, A. M. Rubenchik, M. L. Spaeth, and R. P. Hackel, “Pulse length dependence of laser conditioning and bulk damage in KD2PO4,” Proc. SPIE 5647, 265 (2004).
Damiani, D.
M. Pommiès, D. Damiani, B. Bertussi, J. Capoulade, H. Piombini, J. Y. Natoli, and H. Mathis, “Detection and characterization of absorption heterogeneities in KH2PO4 crystals,” Opt. Commun. 267(1), 154–161 (2006).
[Crossref]
De Yoreo, J.
M. Runkel, M. Yan, J. De Yoreo, and N. Zaitseva, “The effect of impurities and stress on the damage distributions of rapidly grown KDP crystals,” Proc. SPIE 3244, 211 (1997).
M. Runkel, M. Yan, J. De Yoreo, and N. Zaitseva, “The effect of impurities and stress on the damage distributions of rapidly grown KDP crystals,” Proc. SPIE 3244, 211 (1997).
De Yoreo, J. J.
S. G. Demos, M. Staggs, M. Yan, H. B. Radousky, and J. J. De Yoreo, “Investigation of optically active defect clusters in KH2PO4 under laser photoexcitation,” J. Appl. Phys. 85(8), 3988–3992 (1999).
[Crossref]
DeMange, P.
C. W. Carr, J. D. Bude, and P. DeMange, “Lasersupported solidstate absorption fronts in silica,” Phys. Rev. B 82(18), 184304 (2010).
[Crossref]
R. A. Negres, N. P. Zaitseva, P. DeMange, and S. G. Demos, “An expedited approach to evaluate the importance of different crystal growth parameters on laser damage performance in KDP and DKDP,” Proc. SPIE 6403, 64031S (2007).
Demos, S. G.
R. A. Negres, N. P. Zaitseva, P. DeMange, and S. G. Demos, “An expedited approach to evaluate the importance of different crystal growth parameters on laser damage performance in KDP and DKDP,” Proc. SPIE 6403, 64031S (2007).
S. G. Demos, M. Staggs, M. Yan, H. B. Radousky, and J. J. De Yoreo, “Investigation of optically active defect clusters in KH2PO4 under laser photoexcitation,” J. Appl. Phys. 85(8), 3988–3992 (1999).
[Crossref]
DeYoreo, J.
M. Yan, R. Torres, M. Runkel, B. Woods, I. Hutcheon, N. Zaitseva, and J. DeYoreo, “Investigation of impurity and laserinduced damage in the growth sectors of rapidly grown KDP crystals,” Proc. SPIE 2966, 11–16 (1997).
[Crossref]
Dixit, S.
P. Wegner, J. Auerbach, T. Biesiada, S. Dixit, J. Lawson, J. Menapace, T. Parham, D. Swift, P. Whitman, and W. Williams, “NIF final optics systems: frequency conversion and beam conditioning,” Proc. SPIE 5341, 180–189 (2004).
[Crossref]
Feit, M.
J. Adams, J. A. Jarboe, M. Feit, and R. P. Hackel, “Comparison between S/1 and R/1 tests and damage density vs. fluence (rho(phi)) results for unconditioned and subnanosecond laserconditioned KD2PO4 crystals,” Proc. SPIE 6720, 672014 (2008).
Feit, M. D.
C. W. Carr, M. D. Feit, M. C. Nostrand, and J. J. Adams, “Techniques for qualitative and quantitative measurement of aspects of laserinduced damage important for laser beam propagation,” Meas. Sci. Technol. 17(7), 1958–1962 (2006).
[Crossref]
J. B. Trenholme, M. D. Feit, and A. M. Rubenchik, “Sizeselection initiation model extended to include shape and random factors,” Proc. SPIE 5991, 59910X (2005).
[Crossref]
J. J. Adams, C. W. Carr, M. D. Feit, A. M. Rubenchik, M. L. Spaeth, and R. P. Hackel, “Pulse length dependence of laser conditioning and bulk damage in KD2PO4,” Proc. SPIE 5647, 265 (2004).
M. D. Feit and A. M. Rubenchik, “Implications of nanoabsorber initiators for damage probability curves, pulselength scaling and laser conditioning,” Proc. SPIE 5273, 74–82 (2003).
Hackel, R. P.
J. Adams, J. A. Jarboe, M. Feit, and R. P. Hackel, “Comparison between S/1 and R/1 tests and damage density vs. fluence (rho(phi)) results for unconditioned and subnanosecond laserconditioned KD2PO4 crystals,” Proc. SPIE 6720, 672014 (2008).
J. J. Adams, C. W. Carr, M. D. Feit, A. M. Rubenchik, M. L. Spaeth, and R. P. Hackel, “Pulse length dependence of laser conditioning and bulk damage in KD2PO4,” Proc. SPIE 5647, 265 (2004).
Hahn, D.
M. Runkel, J. Bruere, W. Sell, T. Weiland, D. Milam, D. Hahn, and M. Nostrand, “Effects of pulse duration of bulk laser damage in 350nm rasterscanned DKDP,” Proc. SPIE 4392, 405 (2002).
HawleyFedder, R. A.
A. K. Burnham, M. Runkel, R. A. HawleyFedder, M. L. Carman, R. A. Torres, and P. K. Whitman, “Lowtemperature growth of DKDP for improving laserinduced damage resistance at 350nm,” Proc. SPIE 4347, 373 (2000).
Huebel, J.
Z. M. Liao, J. Huebel, J. Trenholme, K. Manes, and C. W. Carr, “Modeling maxofN fluence distribution using measured shottoshot beam contrast,” Appl. Opt. 50(20), 3547–3552 (2011).
[Crossref]
[PubMed]
Hutcheon, I.
M. Yan, R. Torres, M. Runkel, B. Woods, I. Hutcheon, N. Zaitseva, and J. DeYoreo, “Investigation of impurity and laserinduced damage in the growth sectors of rapidly grown KDP crystals,” Proc. SPIE 2966, 11–16 (1997).
[Crossref]
Jarboe, J. A.
J. Adams, J. A. Jarboe, M. Feit, and R. P. Hackel, “Comparison between S/1 and R/1 tests and damage density vs. fluence (rho(phi)) results for unconditioned and subnanosecond laserconditioned KD2PO4 crystals,” Proc. SPIE 6720, 672014 (2008).
Lawson, J.
P. Wegner, J. Auerbach, T. Biesiada, S. Dixit, J. Lawson, J. Menapace, T. Parham, D. Swift, P. Whitman, and W. Williams, “NIF final optics systems: frequency conversion and beam conditioning,” Proc. SPIE 5341, 180–189 (2004).
[Crossref]
Liao, Z. M.
Z. M. Liao, J. Huebel, J. Trenholme, K. Manes, and C. W. Carr, “Modeling maxofN fluence distribution using measured shottoshot beam contrast,” Appl. Opt. 50(20), 3547–3552 (2011).
[Crossref]
[PubMed]
Z. M. Liao, M. L. Spaeth, K. Manes, J. J. Adams, and C. W. Carr, “Predicting laserinduced bulk damage and conditioning for deuterated potassium dihydrogen phosphate crystals using an absorption distribution model,” Opt. Lett. 35(15), 2538–2540 (2010).
[Crossref]
[PubMed]
Manes, K.
Z. M. Liao, J. Huebel, J. Trenholme, K. Manes, and C. W. Carr, “Modeling maxofN fluence distribution using measured shottoshot beam contrast,” Appl. Opt. 50(20), 3547–3552 (2011).
[Crossref]
[PubMed]
Z. M. Liao, M. L. Spaeth, K. Manes, J. J. Adams, and C. W. Carr, “Predicting laserinduced bulk damage and conditioning for deuterated potassium dihydrogen phosphate crystals using an absorption distribution model,” Opt. Lett. 35(15), 2538–2540 (2010).
[Crossref]
[PubMed]
Mathis, H.
M. Pommiès, D. Damiani, B. Bertussi, J. Capoulade, H. Piombini, J. Y. Natoli, and H. Mathis, “Detection and characterization of absorption heterogeneities in KH2PO4 crystals,” Opt. Commun. 267(1), 154–161 (2006).
[Crossref]
Menapace, J.
P. Wegner, J. Auerbach, T. Biesiada, S. Dixit, J. Lawson, J. Menapace, T. Parham, D. Swift, P. Whitman, and W. Williams, “NIF final optics systems: frequency conversion and beam conditioning,” Proc. SPIE 5341, 180–189 (2004).
[Crossref]
Milam, D.
M. Runkel, J. Bruere, W. Sell, T. Weiland, D. Milam, D. Hahn, and M. Nostrand, “Effects of pulse duration of bulk laser damage in 350nm rasterscanned DKDP,” Proc. SPIE 4392, 405 (2002).
J. Swain, S. Stokowski, D. Milam, and F. Rainer, “Improving the bulk laser damage resistance of potassium dihydrogen phosphate crystals by pulsed laser irradiation,” Appl. Phys. Lett. 40(4), 350–352 (1982).
[Crossref]
Natoli, J. Y.
M. Pommiès, D. Damiani, B. Bertussi, J. Capoulade, H. Piombini, J. Y. Natoli, and H. Mathis, “Detection and characterization of absorption heterogeneities in KH2PO4 crystals,” Opt. Commun. 267(1), 154–161 (2006).
[Crossref]
Neeb, K.
M. Runkel, K. Neeb, M. Staggs, J. Auerbach, and A. Burnham, “Results of raster scan laser conditioning studies on DKDP triplers using Nd:YAG and excimer lasers,” Proc. SPIE 4679, 348 (2001).
Negres, R. A.
R. A. Negres, N. P. Zaitseva, P. DeMange, and S. G. Demos, “An expedited approach to evaluate the importance of different crystal growth parameters on laser damage performance in KDP and DKDP,” Proc. SPIE 6403, 64031S (2007).
Nostrand, M.
M. Runkel, J. Bruere, W. Sell, T. Weiland, D. Milam, D. Hahn, and M. Nostrand, “Effects of pulse duration of bulk laser damage in 350nm rasterscanned DKDP,” Proc. SPIE 4392, 405 (2002).
Nostrand, M. C.
C. W. Carr, M. D. Feit, M. C. Nostrand, and J. J. Adams, “Techniques for qualitative and quantitative measurement of aspects of laserinduced damage important for laser beam propagation,” Meas. Sci. Technol. 17(7), 1958–1962 (2006).
[Crossref]
Parham, T.
P. Wegner, J. Auerbach, T. Biesiada, S. Dixit, J. Lawson, J. Menapace, T. Parham, D. Swift, P. Whitman, and W. Williams, “NIF final optics systems: frequency conversion and beam conditioning,” Proc. SPIE 5341, 180–189 (2004).
[Crossref]
Piombini, H.
M. Pommiès, D. Damiani, B. Bertussi, J. Capoulade, H. Piombini, J. Y. Natoli, and H. Mathis, “Detection and characterization of absorption heterogeneities in KH2PO4 crystals,” Opt. Commun. 267(1), 154–161 (2006).
[Crossref]
Pommiès, M.
M. Pommiès, D. Damiani, B. Bertussi, J. Capoulade, H. Piombini, J. Y. Natoli, and H. Mathis, “Detection and characterization of absorption heterogeneities in KH2PO4 crystals,” Opt. Commun. 267(1), 154–161 (2006).
[Crossref]
Radousky, H. B.
S. G. Demos, M. Staggs, M. Yan, H. B. Radousky, and J. J. De Yoreo, “Investigation of optically active defect clusters in KH2PO4 under laser photoexcitation,” J. Appl. Phys. 85(8), 3988–3992 (1999).
[Crossref]
Rainer, F.
J. Swain, S. Stokowski, D. Milam, and F. Rainer, “Improving the bulk laser damage resistance of potassium dihydrogen phosphate crystals by pulsed laser irradiation,” Appl. Phys. Lett. 40(4), 350–352 (1982).
[Crossref]
Rubenchik, A. M.
J. B. Trenholme, M. D. Feit, and A. M. Rubenchik, “Sizeselection initiation model extended to include shape and random factors,” Proc. SPIE 5991, 59910X (2005).
[Crossref]
J. J. Adams, C. W. Carr, M. D. Feit, A. M. Rubenchik, M. L. Spaeth, and R. P. Hackel, “Pulse length dependence of laser conditioning and bulk damage in KD2PO4,” Proc. SPIE 5647, 265 (2004).
M. D. Feit and A. M. Rubenchik, “Implications of nanoabsorber initiators for damage probability curves, pulselength scaling and laser conditioning,” Proc. SPIE 5273, 74–82 (2003).
Runkel, M.
M. Runkel, J. Bruere, W. Sell, T. Weiland, D. Milam, D. Hahn, and M. Nostrand, “Effects of pulse duration of bulk laser damage in 350nm rasterscanned DKDP,” Proc. SPIE 4392, 405 (2002).
M. Runkel, K. Neeb, M. Staggs, J. Auerbach, and A. Burnham, “Results of raster scan laser conditioning studies on DKDP triplers using Nd:YAG and excimer lasers,” Proc. SPIE 4679, 348 (2001).
A. K. Burnham, M. Runkel, R. A. HawleyFedder, M. L. Carman, R. A. Torres, and P. K. Whitman, “Lowtemperature growth of DKDP for improving laserinduced damage resistance at 350nm,” Proc. SPIE 4347, 373 (2000).
M. Runkel and A. K. Burnham, “Difference in bulk damage probability distributions between tripler and zcuts of KDP and DKDP at 355nm,” Proc. SPIE 4347, 408 (2000).
M. Yan, R. Torres, M. Runkel, B. Woods, I. Hutcheon, N. Zaitseva, and J. DeYoreo, “Investigation of impurity and laserinduced damage in the growth sectors of rapidly grown KDP crystals,” Proc. SPIE 2966, 11–16 (1997).
[Crossref]
M. Runkel, M. Yan, J. De Yoreo, and N. Zaitseva, “The effect of impurities and stress on the damage distributions of rapidly grown KDP crystals,” Proc. SPIE 3244, 211 (1997).
M. Runkel, M. Yan, J. De Yoreo, and N. Zaitseva, “The effect of impurities and stress on the damage distributions of rapidly grown KDP crystals,” Proc. SPIE 3244, 211 (1997).
Sell, W.
M. Runkel, J. Bruere, W. Sell, T. Weiland, D. Milam, D. Hahn, and M. Nostrand, “Effects of pulse duration of bulk laser damage in 350nm rasterscanned DKDP,” Proc. SPIE 4392, 405 (2002).
Spaeth, M. L.
Z. M. Liao, M. L. Spaeth, K. Manes, J. J. Adams, and C. W. Carr, “Predicting laserinduced bulk damage and conditioning for deuterated potassium dihydrogen phosphate crystals using an absorption distribution model,” Opt. Lett. 35(15), 2538–2540 (2010).
[Crossref]
[PubMed]
C. W. Carr, J. B. Trenholme, and M. L. Spaeth, “Effect of temporal pulse shape on optical damage,” Appl. Phys. Lett. 90(4), 041110 (2007).
[Crossref]
J. J. Adams, C. W. Carr, M. D. Feit, A. M. Rubenchik, M. L. Spaeth, and R. P. Hackel, “Pulse length dependence of laser conditioning and bulk damage in KD2PO4,” Proc. SPIE 5647, 265 (2004).
Staggs, M.
M. Runkel, K. Neeb, M. Staggs, J. Auerbach, and A. Burnham, “Results of raster scan laser conditioning studies on DKDP triplers using Nd:YAG and excimer lasers,” Proc. SPIE 4679, 348 (2001).
S. G. Demos, M. Staggs, M. Yan, H. B. Radousky, and J. J. De Yoreo, “Investigation of optically active defect clusters in KH2PO4 under laser photoexcitation,” J. Appl. Phys. 85(8), 3988–3992 (1999).
[Crossref]
Stokowski, S.
J. Swain, S. Stokowski, D. Milam, and F. Rainer, “Improving the bulk laser damage resistance of potassium dihydrogen phosphate crystals by pulsed laser irradiation,” Appl. Phys. Lett. 40(4), 350–352 (1982).
[Crossref]
Swain, J.
J. Swain, S. Stokowski, D. Milam, and F. Rainer, “Improving the bulk laser damage resistance of potassium dihydrogen phosphate crystals by pulsed laser irradiation,” Appl. Phys. Lett. 40(4), 350–352 (1982).
[Crossref]
Swift, D.
P. Wegner, J. Auerbach, T. Biesiada, S. Dixit, J. Lawson, J. Menapace, T. Parham, D. Swift, P. Whitman, and W. Williams, “NIF final optics systems: frequency conversion and beam conditioning,” Proc. SPIE 5341, 180–189 (2004).
[Crossref]
Torres, R.
M. Yan, R. Torres, M. Runkel, B. Woods, I. Hutcheon, N. Zaitseva, and J. DeYoreo, “Investigation of impurity and laserinduced damage in the growth sectors of rapidly grown KDP crystals,” Proc. SPIE 2966, 11–16 (1997).
[Crossref]
Torres, R. A.
A. K. Burnham, M. Runkel, R. A. HawleyFedder, M. L. Carman, R. A. Torres, and P. K. Whitman, “Lowtemperature growth of DKDP for improving laserinduced damage resistance at 350nm,” Proc. SPIE 4347, 373 (2000).
Trenholme, J.
Z. M. Liao, J. Huebel, J. Trenholme, K. Manes, and C. W. Carr, “Modeling maxofN fluence distribution using measured shottoshot beam contrast,” Appl. Opt. 50(20), 3547–3552 (2011).
[Crossref]
[PubMed]
Trenholme, J. B.
C. W. Carr, J. B. Trenholme, and M. L. Spaeth, “Effect of temporal pulse shape on optical damage,” Appl. Phys. Lett. 90(4), 041110 (2007).
[Crossref]
J. B. Trenholme, M. D. Feit, and A. M. Rubenchik, “Sizeselection initiation model extended to include shape and random factors,” Proc. SPIE 5991, 59910X (2005).
[Crossref]
Wegner, P.
P. Wegner, J. Auerbach, T. Biesiada, S. Dixit, J. Lawson, J. Menapace, T. Parham, D. Swift, P. Whitman, and W. Williams, “NIF final optics systems: frequency conversion and beam conditioning,” Proc. SPIE 5341, 180–189 (2004).
[Crossref]
Weiland, T.
M. Runkel, J. Bruere, W. Sell, T. Weiland, D. Milam, D. Hahn, and M. Nostrand, “Effects of pulse duration of bulk laser damage in 350nm rasterscanned DKDP,” Proc. SPIE 4392, 405 (2002).
Whitman, P.
P. Wegner, J. Auerbach, T. Biesiada, S. Dixit, J. Lawson, J. Menapace, T. Parham, D. Swift, P. Whitman, and W. Williams, “NIF final optics systems: frequency conversion and beam conditioning,” Proc. SPIE 5341, 180–189 (2004).
[Crossref]
Whitman, P. K.
A. K. Burnham, M. Runkel, R. A. HawleyFedder, M. L. Carman, R. A. Torres, and P. K. Whitman, “Lowtemperature growth of DKDP for improving laserinduced damage resistance at 350nm,” Proc. SPIE 4347, 373 (2000).
Williams, W.
P. Wegner, J. Auerbach, T. Biesiada, S. Dixit, J. Lawson, J. Menapace, T. Parham, D. Swift, P. Whitman, and W. Williams, “NIF final optics systems: frequency conversion and beam conditioning,” Proc. SPIE 5341, 180–189 (2004).
[Crossref]
Woods, B.
M. Yan, R. Torres, M. Runkel, B. Woods, I. Hutcheon, N. Zaitseva, and J. DeYoreo, “Investigation of impurity and laserinduced damage in the growth sectors of rapidly grown KDP crystals,” Proc. SPIE 2966, 11–16 (1997).
[Crossref]
Yan, M.
S. G. Demos, M. Staggs, M. Yan, H. B. Radousky, and J. J. De Yoreo, “Investigation of optically active defect clusters in KH2PO4 under laser photoexcitation,” J. Appl. Phys. 85(8), 3988–3992 (1999).
[Crossref]
M. Yan, R. Torres, M. Runkel, B. Woods, I. Hutcheon, N. Zaitseva, and J. DeYoreo, “Investigation of impurity and laserinduced damage in the growth sectors of rapidly grown KDP crystals,” Proc. SPIE 2966, 11–16 (1997).
[Crossref]
M. Runkel, M. Yan, J. De Yoreo, and N. Zaitseva, “The effect of impurities and stress on the damage distributions of rapidly grown KDP crystals,” Proc. SPIE 3244, 211 (1997).
M. Runkel, M. Yan, J. De Yoreo, and N. Zaitseva, “The effect of impurities and stress on the damage distributions of rapidly grown KDP crystals,” Proc. SPIE 3244, 211 (1997).
Zaitseva, N.
M. Runkel, M. Yan, J. De Yoreo, and N. Zaitseva, “The effect of impurities and stress on the damage distributions of rapidly grown KDP crystals,” Proc. SPIE 3244, 211 (1997).
M. Yan, R. Torres, M. Runkel, B. Woods, I. Hutcheon, N. Zaitseva, and J. DeYoreo, “Investigation of impurity and laserinduced damage in the growth sectors of rapidly grown KDP crystals,” Proc. SPIE 2966, 11–16 (1997).
[Crossref]
M. Runkel, M. Yan, J. De Yoreo, and N. Zaitseva, “The effect of impurities and stress on the damage distributions of rapidly grown KDP crystals,” Proc. SPIE 3244, 211 (1997).
Zaitseva, N. P.
R. A. Negres, N. P. Zaitseva, P. DeMange, and S. G. Demos, “An expedited approach to evaluate the importance of different crystal growth parameters on laser damage performance in KDP and DKDP,” Proc. SPIE 6403, 64031S (2007).
Appl. Opt. (1)
Z. M. Liao, J. Huebel, J. Trenholme, K. Manes, and C. W. Carr, “Modeling maxofN fluence distribution using measured shottoshot beam contrast,” Appl. Opt. 50(20), 3547–3552 (2011).
[Crossref]
[PubMed]
Appl. Phys. Lett. (2)
C. W. Carr, J. B. Trenholme, and M. L. Spaeth, “Effect of temporal pulse shape on optical damage,” Appl. Phys. Lett. 90(4), 041110 (2007).
[Crossref]
J. Swain, S. Stokowski, D. Milam, and F. Rainer, “Improving the bulk laser damage resistance of potassium dihydrogen phosphate crystals by pulsed laser irradiation,” Appl. Phys. Lett. 40(4), 350–352 (1982).
[Crossref]
J. Appl. Phys. (1)
S. G. Demos, M. Staggs, M. Yan, H. B. Radousky, and J. J. De Yoreo, “Investigation of optically active defect clusters in KH2PO4 under laser photoexcitation,” J. Appl. Phys. 85(8), 3988–3992 (1999).
[Crossref]
Meas. Sci. Technol. (1)
C. W. Carr, M. D. Feit, M. C. Nostrand, and J. J. Adams, “Techniques for qualitative and quantitative measurement of aspects of laserinduced damage important for laser beam propagation,” Meas. Sci. Technol. 17(7), 1958–1962 (2006).
[Crossref]
Opt. Commun. (1)
M. Pommiès, D. Damiani, B. Bertussi, J. Capoulade, H. Piombini, J. Y. Natoli, and H. Mathis, “Detection and characterization of absorption heterogeneities in KH2PO4 crystals,” Opt. Commun. 267(1), 154–161 (2006).
[Crossref]
Opt. Lett. (1)
Z. M. Liao, M. L. Spaeth, K. Manes, J. J. Adams, and C. W. Carr, “Predicting laserinduced bulk damage and conditioning for deuterated potassium dihydrogen phosphate crystals using an absorption distribution model,” Opt. Lett. 35(15), 2538–2540 (2010).
[Crossref]
[PubMed]
Phys. Rev. B (1)
C. W. Carr, J. D. Bude, and P. DeMange, “Lasersupported solidstate absorption fronts in silica,” Phys. Rev. B 82(18), 184304 (2010).
[Crossref]
Proc. SPIE (13)
M. D. Feit and A. M. Rubenchik, “Implications of nanoabsorber initiators for damage probability curves, pulselength scaling and laser conditioning,” Proc. SPIE 5273, 74–82 (2003).
J. B. Trenholme, M. D. Feit, and A. M. Rubenchik, “Sizeselection initiation model extended to include shape and random factors,” Proc. SPIE 5991, 59910X (2005).
[Crossref]
M. Runkel, M. Yan, J. De Yoreo, and N. Zaitseva, “The effect of impurities and stress on the damage distributions of rapidly grown KDP crystals,” Proc. SPIE 3244, 211 (1997).
M. Runkel, J. Bruere, W. Sell, T. Weiland, D. Milam, D. Hahn, and M. Nostrand, “Effects of pulse duration of bulk laser damage in 350nm rasterscanned DKDP,” Proc. SPIE 4392, 405 (2002).
J. Adams, J. A. Jarboe, M. Feit, and R. P. Hackel, “Comparison between S/1 and R/1 tests and damage density vs. fluence (rho(phi)) results for unconditioned and subnanosecond laserconditioned KD2PO4 crystals,” Proc. SPIE 6720, 672014 (2008).
R. A. Negres, N. P. Zaitseva, P. DeMange, and S. G. Demos, “An expedited approach to evaluate the importance of different crystal growth parameters on laser damage performance in KDP and DKDP,” Proc. SPIE 6403, 64031S (2007).
M. Runkel, M. Yan, J. De Yoreo, and N. Zaitseva, “The effect of impurities and stress on the damage distributions of rapidly grown KDP crystals,” Proc. SPIE 3244, 211 (1997).
M. Yan, R. Torres, M. Runkel, B. Woods, I. Hutcheon, N. Zaitseva, and J. DeYoreo, “Investigation of impurity and laserinduced damage in the growth sectors of rapidly grown KDP crystals,” Proc. SPIE 2966, 11–16 (1997).
[Crossref]
J. J. Adams, C. W. Carr, M. D. Feit, A. M. Rubenchik, M. L. Spaeth, and R. P. Hackel, “Pulse length dependence of laser conditioning and bulk damage in KD2PO4,” Proc. SPIE 5647, 265 (2004).
M. Runkel, K. Neeb, M. Staggs, J. Auerbach, and A. Burnham, “Results of raster scan laser conditioning studies on DKDP triplers using Nd:YAG and excimer lasers,” Proc. SPIE 4679, 348 (2001).
M. Runkel and A. K. Burnham, “Difference in bulk damage probability distributions between tripler and zcuts of KDP and DKDP at 355nm,” Proc. SPIE 4347, 408 (2000).
A. K. Burnham, M. Runkel, R. A. HawleyFedder, M. L. Carman, R. A. Torres, and P. K. Whitman, “Lowtemperature growth of DKDP for improving laserinduced damage resistance at 350nm,” Proc. SPIE 4347, 373 (2000).
P. Wegner, J. Auerbach, T. Biesiada, S. Dixit, J. Lawson, J. Menapace, T. Parham, D. Swift, P. Whitman, and W. Williams, “NIF final optics systems: frequency conversion and beam conditioning,” Proc. SPIE 5341, 180–189 (2004).
[Crossref]
Other (1)
M. Spaeth, “Absorption distribution model,” LLNL Internal Presentation (2007).
Cited By
OSA participates in Crossref's CitedBy Linking service. Citing articles from OSA journals and other participating publishers are listed here.
Alert me when this article is cited.
Figures (8)
Schematic of a DKDP boule with growth regions and an illustration of precursor defects with different sizes (a) and densities (α). Filledin circles denote Type 1 precursors and open circles denote Type 2 precursors (see theory section).
Damage probability measurement (S/1circle, R/1filled dot) (a) and corresponding parameters of Type 1 and Type 2 absorption distribution as extracted by ADM model (b).
Damage density ρ(ϕ) measurement with ADM prediction (a) and corresponding precursor density distribution used by ADM (b).
Defect parameter histogram for absorption mean (μ) on left (a) and for absorption standard deviation (σ) on (b) for both Type 1 (filled) and Type 2 (notfilled) precursor types.
(a) Plot of Type 1 vs. Type 2 absorption parameters (mean, μ  open symbol, standard deviation, σ  filled symbol) for all data on all boules. (b) grouped plot of Type 1 vs. Type 2 absorption parameter for FG (circle) and LG for LL16 boule only.
Plot of Type 1 vs. Type 2 defect mean absorption for each boule and the relationship between the FG and LG as indicated by the direction of the arrow.
Type 1 defect mean absorption (μ_{1}) vs. precursor density N for Group A boules (data – circular blue, fit blue line) and Group B boules (data – red square, fit red line). Data from ungrouped boules (lack of LG data) were marked as green triangles.
Contour plot of the conditioning map showing the number of damage initiations (in log units) for a nominal boule from Group A (left graph) vs. the worst outlier boule from Group B (right graph), the optimal conditioning sequence to reach 8 J/cm^{2} for each boule is shown in red solid line.
Tables (1)
Table 1 Boule samples with various damage testing data
Equations (6)
Equations on this page are rendered with MathJax. Learn more.